International Journal of Photoenergy

Volume 2014 (2014), Article ID 146892, 7 pages

http://dx.doi.org/10.1155/2014/146892

Research Article

Controllable Fabrication of Ordered Mesoporous Bi₂WO₆ and Its High Photocatalytic Activity under Visible Light

Xueming Dang,¹ Xiaoli Dong,¹ Hua Wang,² Xiufang Zhang,¹ Hongchao Ma,¹ and Mang Xue¹

¹School of Light Industry and Chemical Engineering, Dalian Polytechnic University, Dalian 116034, China

²College of Fisheries and Life Science, Dalian Ocean University, Dalian 116023, China

Received 17 April 2014; Revised 17 June 2014; Accepted 18 June 2014; Published 26 June 2014

Academic Editor: Yuexiang Li

Copyright © 2014 Xueming Dang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Ordered mesoporous Bi₂WO₆ was fabricated by nanocasting technique using SBA-15 as the template. The effect of the dosage of SBA-15 on the formation of the ordered structure and the photocatalytic ability of mesoporous Bi₂WO₆ was discussed. It was confirmed that the ordered mesoporous structure was obtained as the dosage of SBA-15 was 0.3 g. It was found that, compared to Bi₂WO₆, the RhB degradation rate with ordered mesoporous Bi₂WO₆ was enhanced under visible light ( nm) by the photocatalytic measurements. The enhanced photocatalytic performance of ordered mesoporous Bi₂WO₆ was attributed to its particular ordered mesoporous structure which could increase the light-harvesting efficiency, reduce the recombination of the photogenerated charge carriers, and promote the surface reaction.

1. Introduction

Photocatalytic degradation of organic compounds for the purpose of purifying wastewater from industries and households has attracted much attention in recent years [1]. Heterogeneous photocatalysis is a common advanced oxidation approach for the removal of hazardous organic compounds from wastewater [2–4]. Photocatalysts can harness solar energy to drive useful redox chemistry and therefore are of considerable interest for environmental pollutant treatment [5–7]. Recently, the research of visible-light-driven photocatalysts has drawn the interest of a number of researchers [8–10]. Bi₂WO₆, with a narrow band gap of 2.7 eV is one of the most attractive materials because of its high stability, nontoxicity, and wide solar response [11–13]. However, just as other photocatalysts, it suffers from the low quantum efficiency. Therefore, some attempts have been devoted to improve the photocatalytic performance of Bi₂WO₆ [14, 15].

Porous materials are of great interest in the application in photocatalysis, owing to their high surface area, which is a basic requirement for an efficient photocatalyst both to enhance the adsorption of photos and reactants and to offer a large number of reactive sites [16–18]. An ordered porous structure is highly desirable for effective photocatalysis due to their larger surface area and multiple aligned pores, which can further assist the electron/energy transfer within the porous framework [19–22].

The nanocasting pathways developed over the last ten years, which use hard templates to create ordered replicas and provide promising routes for the preparation of mesostructured materials with novel framework compositions. Yang et al. [23–25] have demonstrated that ordered mesoporous silicas, such as two-dimensional (2D) hexagonal (p6 mm) SBA-15 and three-dimensional (3D) bicontinuous cubic (Ia3d) KIT-6, can be used as a hard template to fabricate various ordered crystalline metal oxides. Nanocasting is processed by filling the void of the template with a precursor of the material, subsequent transform of the precursor to the material, and final removal of the template; a replica structure can be obtained [26]. The quantity rate of template to the precursor can affect the structure and the morphology of the materials.

Herein, taking SBA-15 as the template, ordered mesoporous Bi₂WO₆ was fabricated by nanocasting technique to get enhanced photocatalytic ability under visible light. The effect of the dosage of SBA-15 on the formation of the ordered structure and the photocatalytic ability of mesoporous Bi₂WO₆ was discussed. RhB, a common pollutant in the industry wastewater, was chosen as a test substance to evaluate the photocatalytic performance of the as-prepared samples under visible light.

2. Materials and Methods

2.1. Materials

Tetraethyl orthosilicate (TEOS) was used as the silica source and poly(ethylene glycol)-block-poly(propylene glycol)-block-poly(ethylene glycol) (P123) was used as the surfactant for the preparation of SBA-15. Bismuth (III) nitrate pentahydrate (Bi(NO₃)₃·5H₂O) and sodium tungstate dehydrate (Na₂WO₆·2H₂O) were used as the bismuth source and the tungsten source, respectively. All reagents were of analytical grade and were used as received.

2.2. Methods

2.2.1. Preparation of Mesoporous Silica SBA-15

The preparation process of SBA-15 referred to the method reported by Zhao and coworkers [27]. About 2 g of P123 was dissolved with 50 mL of deionized water at 35°C followed by addition of 55 g of 4 mol/L HCl solution. After P123 was fully dissolved 4 g of TEOS was added into the solution drop by drop (TEOS : P123 : HCl : H₂O = 1 : 0.017 : 9.861 : 137). The mixture was stirred at 35°C for 24 h before transferring into a Teflon bottle sealed in an autoclave, which was then heated to 100°C for 48 h in an oven. The solid was filtered off, washed three times with deionized water, dried at 100°C for 6 h, and calcined at 600°C for 6 h.

2.2.2. Preparation of Ordered Mesoporous Bi₂WO₆

Under ultrasonication, 4 mmol of Bi(NO₃)₃·5H₂O was dissolved in 20 mL of 2 M HNO₃ solution, and then a transparent colorless solution was obtained. Followed 2 mmol Na₂WO₄·2H₂O was added to the solution under ultrasonication for 10 min to form a white solution. Then a certain amount of prepared SBA-15 was added. The samples with 0.15 g, 0.3 g, and 0.6 g of SBA-15 were recorded by S₁, S2, and S₃, respectively. After complete immersion of the SBA-15, the mixture was put into the electrothermal constant-temperature dry box at 65°C for 18 h to complete filling the Bi₂WO₆ precursor into the void of SBA-15. The dried sample was then converted by calcination at 400°C for 6 h. Finally, the ordered mesoporous Bi₂WO₆ product was obtained with 20 mL of 2 M NaOH solution for 6 h under ambient temperature to eliminate SBA-15. The final product was filtered and washed with distilled water and absolute ethanol. Moreover, the Bi₂WO₆ was obtained as the same process without the addition and removal of SBA-15.

2.2.3. Sample Characterization

Low-angle X-ray diffraction (LXRD) and wide-angle X-ray diffraction (WXRD) spectra were recorded by Rigaku D/MAX-2400 with Cu Ka radiation, accelerating voltage of 40 kV, and current of 30 mA. The scanning rate was 8° () min⁻¹ and the scanning range was 10–80°. Light absorption properties were determined using a UV-vis spectrophotometer (Shimadzu, UV-2450) with a wavelength range of 200–800 nm. The micromorphologies of the samples were observed using a transmission electron microscopy (TEM, JEM-2100(UHR) JEOL). TriStar 3000 was used to examine the N₂ adsorption and desorption properties of the samples at −196°C. Specific surface areas were calculated via the Brunauer-Emmett-Teller (BET) model. Fluorescence (FL) spectra were recorded by fluorescence spectrometer (LS-55, PE).

2.2.4. Measurement of Photocatalytic Activity

The photocatalytic activities of the samples were monitored through the photodegradation of RhB under visible light irradiation. Photocatalytic reactions were conducted in a 100 mL cubic quartz reactor. A 300 W Xe lamp was employed as visible light source. The light was passed through a filter, which should shield any wavelength below 400 nm. In all experiments, the photocatalyst (0.10 g) was added to 100 mL RhB aqueous solution (5 mg/L). During each photocatalytic experiment, 5 mL of the suspension was collected at predetermined time intervals. The suspension was centrifuged at 9500 rpm for 10 min, and the concentration of RhB in the supernatant was analyzed by measuring the absorbance at 553 nm with a Shimadzu UV2000 spectrophotometer.

3. Results and Discussion

3.1. XRD Analysis

The measurements of WXRD and LXRD patterns were performed to identify the crystalline phase and mesoporous ordering of as-prepared samples (see Figure 1). The WXRD patterns of Bi₂WO₆, S₁, S2, and S₃ were shown in Figure 1(a). The crystal forms of the Bi₂WO₆ and mesoporous Bi₂WO₆ could be identified to the orthorhombic type according to JCPDS card number 73-2020. And no other peaks were found in the spectra of S₁, S2, and S₃, indicating that no other crystal type was formed, and the template of SBA-15 was completely removed. One obvious peak ( 0.80°) and a little peak ( 0.98°) in the LXRD pattern of S₂ could be found, inferring that the periodically ordered structure of S₂ was obtained. However, no ordered mesoporous Bi₂WO₆ was found in S₁ and S₃, based on the result that there were no obvious peaks in the LXRD spectra of them. The results indicated that the dosage of SBA-15 could affect the formation of the ordered mesoporous structure.

(a)

(b)

Figure 1: (a) WXRD patterns of Bi₂WO₆, S₁ S₂, and S₃ and (b) LXRD patterns of S₁, S₂, and S₃.

3.2. Nitrogen Adsorption-Desorption and TEM Analysis

N₂ sorption isotherms and pore size distributions (inset) of the Bi₂WO₆, SBA-15, S₁, S2, and S₃ were displayed in Figure 2. The N₂ adsorption/desorption curve of SBA-15 showed a typical type IV isotherm with the hysteresis loop. Sharp capillary condensation over a narrow relative pressure region indicated the high degree of ordering, corresponding to a mesopore size of 7.7 nm. The SBA-15 had a surface area of 541.8 m²/g and a pore volume of 0.75 cm³/g. The isotherms of S₁, S2, and S₃ showed also a type IV curve, indicating a porous feature as shown in Figure 2. And the degree of ordering of S₂ (pore size of 5.1 nm) was higher than that of S₁ and S₃ based on the relative pressure regions of capillary condensation, which was the same as the result of LXRD. Furthermore, the particle size of Bi₂WO₆ based on TEM image was about 100–200 nm. The big particle and nonporous structure leaded to low surface area of Bi₂WO₆ (20.5 m²/g), which was lower than those of S₁ (38.6 m²/g), S₂ (66.7 m²/g), and S₃ (25.5 m²/g). Large surface area could provide more sites for promoted surface reaction.

Figure 2: N2 sorption isotherms and pore size distributions (inset) of the Bi₂WO₆, SBA-15, S₁, S2, and S₃.

The ordering degrees of S₁, S2, and S₃ got by the analysis of LXRD were certified by TEM images (Figure 3). No ordered structure was found in S₁ and S₃, but ordered replicas of SBA-15 were found in S₂. The HRTEM image of S₂ was presented in Figure 3(f). It could be measured that the spacing was 0.320 nm, which matched well to the lattice spacing of (113) of orthorhombic type Bi₂WO₆ according to JCPDS card number 73-2020. Furthermore, some big particles with nonporous structure were found in S₁, and there were some larger pores in S₃. The ordered porosity of the S₂ resulted from interparticle voids. In the filling process, the pores of SBA-15 were completely filled. After the template was removed, the interparticle would construct the ordered mesoporous structure. SBA-15 dosage of S₁ was only 0.15 g, which was lack of enough pores to make the Bi₂WO₆ particles highly be organized. As a result some particles gathered together. And for the S₃ with 0.6 g SBA-15, there were too much pores for the precursor of Bi₂WO₆ to permeate. The distance of the particles would be larger than the pore size of SBA-15. The Bi₂WO₆ particles maybe gathered after the template was removed. So many pores may make the Bi₂WO₆ arrange irregularly.

Figure 3: TEM image of (a) SBA-15, (b) Bi₂WO₆, (c) S₁, (d) S₃, and (e) S₂ and (f) the HRTEM image of S₂.

3.3. Optical Absorption Ability

The photo absorption abilities of the samples were detected by UV-vis absorption spectra, and the results were shown in Figure 4(a). All the samples showed intense absorption in the region from 200 to 450 nm. An obvious red shift of band gap edge was found in the spectra of mesoporous Bi₂WO₆. The band gaps of Bi₂WO₆ and S₂ were determined to be 2.72 and 2.59 eV, respectively (Figure 4(b)), according to the Kubelka-Munk function

(a)

(b)

Figure 4: (a) UV-vis absorption spectra of Bi₂WO₆, S₁, S2, and S3 and (b) calculation of the band gap by Bi₂WO₆ and S₂ by Kubelka-Munk function.

Because Bi₂WO₆ is the directly allowed optical transition semiconductor, in the function equals 1. The narrower band gap of S₂ meant that S₂ could be excited by more photos and had enhanced light absorption ability.

3.4. FL Spectra Analysis

FL analysis was used to reveal the separation efficiency of the photogenerated electrons and holes in semiconductors, and the results were shown in Figure 5. The lower peak indicated lower recombination rate of them. The FL intensity of Bi₂WO₆ was the biggest one, inferring that Bi₂WO₆ had the highest recombination rate of photogenerated charge carriers. The results confirmed that the separation of photogenerated charge carriers could be improved through the construction of mesoporous Bi₂WO₆, leading to the enhancement of photocatalytic activity. The FL intensity of S₂ got the lowest one among those of mesoporous Bi₂WO₆, indicating that S₂ should have higher photocatalytic ability.

Figure 5: FL spectra of Bi₂WO₆, S₁, S₂, and S₃.

3.5. Photocatalytic Activity

The variation of RhB concentration (), where was the concentration of RhB at irradiation time () and is the initial concentration of RhB (5 mg/L) versus over the photocatalysts, was shown in Figure 6(a). In 30 min, only 23.8% of RhB was removed with Bi₂WO₆. However, RhB removal rate with S₁, S₂, and S₃ was 69.2%, 91.5%, and 39.0%, respectively. The results indicated that the photocatalytic ability of Bi₂WO₆ could be enhanced by constructing mesoporous structure. And the photocatalytic ability of S₂ was higher than those of S₁ and S₃, inferring that the ordered mesoporous structure could further enhance the photocatalytic performance of Bi₂WO₆. Because of the ordered mesoporous structure, the harvesting of incident light of S₂ became more efficient; the separation efficiency of photogenerated charge carriers was enhanced. Thus, an increased number of electrons and holes would arrive at the surface of Bi₂WO₆ particles, participating in oxidative reactions with RhB. High surface area could also provide more active sites for oxidative reactions and subsequently promote RhB removal. The adsorption performance of RhB of S₂ was measured, and the result has been presented in Figure 6(b). The removal rate of RhB (26.0%) was largely lower than that in photocatalytic process, indicating that ordered mesoporous Bi₂WO₆ had excellent photocatalytic ability.

(a)

(b)

Figure 6: Ct/C₀ of the RhB concentration versus reaction time for (a) photocatalytic degradation with Bi₂WO₆, S₁, S₂, and S₃ under visible light and (b) adsorption with S₂.

4. Conclusions

Ordered mesoporous Bi₂WO₆ was successfully synthesized by nanocasting technique using SBA-15 as the template. The dosage of SBA-15 could affect the formation of ordered structure of mesoporous Bi₂WO₆. The as-prepared ordered mesoporous Bi₂WO₆ exhibited an excellent photocatalytic decomposition of RhB under visible light irradiation. The high photocatalytic activity could be ascribed to its particularly ordered mesoporous structure which could increase the light-harvesting efficiency, reduce the recombination of the photogenerated charge carriers, and promote the surface reaction. Based on the results got here, it is confirmed that construction of ordered mesoporous structure can efficiently improve the photocatalytic performance of photocatalysts, and photocatalysts with ordered mesoporous structure will be a promising candidate for the removal of hazardous organic compounds from wastewater.

Conflict of Interests

The authors declare that there is no conflict of interests regarding the publication of this paper.

Acknowledgments

This work was supported by the National Science Fund China (Project no. 21107007) and the Program for Liaoning Excellent Talents in University (LJQ2012049).

References

L. Zhang and Y. Zhu, “A review of controllable synthesis and enhancement of performances of bismuth tungstate visible-light-driven photocatalysts,” Catalysis Science and Technology, vol. 2, no. 4, pp. 694–706, 2012.

D. F. Ollis, E. Pelizzetti, and N. Serpone, “Photocatalyzed destruction of water contaminants,” Environmental Science & Technology, vol. 25, no. 9, pp. 1522–1529, 1991.

M. R. Hoffmann, S. T. Martin, W. Choi, and D. W. Bahnemann, “Environmental applications of semiconductor photocatalysis,” Chemical Reviews, vol. 95, no. 1, pp. 69–96, 1995.

L. Liu, H. Liu, Y. Zhao et al., “Directed synthesis of hierarchical nanostructured TiO₂ catalysts and their morphology-dependent photocatalysis for phenol degradation,” Environmental Science and Technology, vol. 42, no. 7, pp. 2342–2348, 2008.

Y. C. Zhang, J. Li, and H. Y. Xu, “One-step in situ solvothermal synthesis of SnS₂/TiO₂ nanocomposites with high performance in visible light-driven photocatalytic reduction of aqueous Cr(VI),” Applied Catalysis B Environmental, vol. 123-124, pp. 18–26, 2012.

Y. C. Zhang, J. Li, M. Zhang, and D. D. Dionysiou, “Size-tunable hydrothermal synthesis of SnS 2 nanocrystals with high performance in visible light-driven photocatalytic reduction of aqueous Cr(VI),” Environmental Science and Technology, vol. 45, no. 21, pp. 9324–9331, 2011.

N. Kajiwara, Y. Noma, and H. Takigami, “Photolysis studies of technical decabromodiphenyl ether (DecaBDE) and ethane (DeBDethane) in plastics under natural sunlight,” Environmental Science and Technology, vol. 42, no. 12, pp. 4404–4409, 2008.

Z. Zou, J. Ye, K. Sayama, and H. Arakawa, “Direct splitting of water under visible light irradiation with an oxide semiconductor photocatalyst,” Nature, vol. 414, no. 6864, pp. 625–627, 2001.

Y. X. Li, J. X. Wang, S. Q. Peng, G. X. Lu, and S. B. Li, “Photocatalytic hydrogen generation in the presence of glucose over ZnS-coated ZnIn₂S₄ under visible light irradiation,” International Journal of Hydrogen Energy, vol. 35, no. 13, pp. 7116–7126, 2010.

Y. X. Li, Y. Jiang, S. Q. Peng, and F. Jiang, “Nitrogen-doped TiO₂ modified with NH4F for efficient photocatalytic degradation of formaldehyde under blue light-emitting diodes,” Journal of Hazardous Materials, vol. 182, no. 1–3, pp. 90–96, 2010.

X. Zhao, T. Xu, W. Yao, C. Zhang, and Y. Zhu, “Photoelectrocatalytic degradation of 4-chlorophenol at Bi₂WO₆ nanoflake film electrode under visible light irradiation,” Applied Catalysis B: Environmental, vol. 72, no. 1-2, pp. 92–97, 2007.

H. Fu, L. Zhang, W. Yao, and Y. Zhu, “Photocatalytic properties of nanosized Bi₂WO₆ catalysts synthesized via a hydrothermal process,” Applied Catalysis B: Environmental, vol. 66, no. 1-2, pp. 100–110, 2006.

H. B. Fu, S. C. Zhang, T. G. Xu, Y. F. Zhu, and J. M. Chen, “Photocatalytic degradation of RhB by fluorinated Bi₂WO₆ and distributions of the intermediate products,” Environmental Science & Technology, vol. 42, no. 6, pp. 2085–2091, 2008.

J. Ren, W. Wang, S. Sun, L. Zhang, and J. Chang, “Enhanced photocatalytic activity of Bi₂WO₆ loaded with Ag nanoparticles under visible light irradiation,” Applied Catalysis B: Environmental, vol. 92, no. 1-2, pp. 50–55, 2009.

M. Ge, Y. Li, L. Liu, Z. Zhou, and W. Chen, “Bi₂O₃-Bi₂WO₆ composite microspheres: hydrothermal synthesis and photocatalytic performances,” The Journal of Physical Chemistry C, vol. 115, no. 13, pp. 5220–5225, 2011.

X. Wang, J. C. Yu, C. Ho, Y. Hou, and X. Fu, “Photocatalytic activity of a hierarchically macro/mesoporous titania,” Langmuir, vol. 21, no. 6, pp. 2552–2559, 2005.

Y. Chen, S. Lunsford, and D. D. Dionysiou, “Photocatalytic activity and electrochemical response of titania film with macro/mesoporous texture,” Thin Solid Films, vol. 516, no. 21, pp. 7930–7936, 2008.

D. G. Shchukin, J. H. Schattka, M. Antonietti, and R. A. Caruso, “Photocatalytic properties of porous metal oxide networks formed by nanoparticle infiltration in a polymer gel template,” Journal of Physical Chemistry B, vol. 107, no. 4, pp. 952–957, 2003.

G. S. Li, D. Q. Zhang, and J. C. Yu, “Ordered mesoporous BiVO₄ through nanocasting: a superior visible light-driven photocatalyst,” Chemistry of Materials, vol. 20, no. 12, pp. 3983–3992, 2008.

S. M. Sun, W. Z. Wang, and L. Zhang, “Facile preparation of three-dimensionally ordered macroporous Bi₂WO₆ with high photocatalytic activity,” Journal of Materials Chemistry, vol. 22, no. 36, pp. 19244–19249, 2012.

L. Dong, X. Zhang, X. Dong et al., “Structuring porous “sponge-like” BiVO₄ film for efficient photocatalysis under visible light illumination,” Journal of Colloid and Interface Science, vol. 393, no. 1, pp. 126–129, 2013.

H. Shibata, T. Ogura, T. Mukai, T. Ohkubo, and H. Sakai, “Direct synthesis of mesoporous titania particles having a crystalline wall,” Journal of the American Chemical Society, vol. 127, no. 47, pp. 16396–16397, 2005.

H. F. Yang, Q. H. Shi, B. Z. Tian et al., “One-step nanocasting synthesis of highly ordered single crystalline indium oxide nanowire arrays from mesostructured frameworks,” Journal of the American Chemical Society, vol. 125, no. 16, pp. 4724–4725, 2003.

B. Tian, X. Liu, H. Yang et al., “General synthesis of ordered crystallized metal oxide nanoarrays replicated by microwave-digested mesoporous silica,” Advanced Materials, vol. 15, no. 16, pp. 1370–1374, 2003.

B. Tian, X. Liu, L. A. Solovyov et al., “Facile synthesis and characterization of novel mesoporous and mesorelief oxides with gyroidal structures,” Journal of the American Chemical Society, vol. 126, no. 3, pp. 865–875, 2004.

A. Lu and F. Schüth, “Nanocasting: a versatile strategy for creating nanostructured porous materials,” Advanced Materials, vol. 18, no. 14, pp. 1793–1805, 2006.

D. Y. Zhao, J. Y. Sun, Q. Z. Li, and G. D. Stucky, “Morphological control of highly ordered mesoporous silica SBA-15,” Chemistry of Materials, vol. 12, no. 2, pp. 275–279, 2000.